Journal of Electrostatics 72 (2014) 396e401
Contents lists available at ScienceDirect
Journal of Electrostatics journal homepage: www.elsevier.com/locate/elstat
An alternative approach for charge decay measurement to assess the suitability of materials John Chubb Infostatic, 2 Monica Drive, Pittville, Cheltenham GL50 4NQ, UK
a r t i c l e i n f o
a b s t r a c t
Article history: Received 31 March 2014 Accepted 16 June 2014 Available online 14 July 2014
A method of charge decay testing is proposed in which a localized electric ﬁeld is applied by a ﬁeldmeter to an area of the material to be tested. The variation of electric ﬁeld is recorded as charge migrates across the surface. Arrangements are described for this method of testing and studies reported comparing results with corona and tribocharge decay measurements. Interesting differences are shown between the methods of testing. Induction charge decay testing is not proposed as a replacement for corona or tribocharge decay testing. It offers the opportunity for simpler instrumentation and measurement of faster charge decay times. © 2014 Elsevier B.V. All rights reserved.
Keywords: Charge decay testing Assessment of materials Measuring instrumentation
1. Introduction The measurement of charge dissipation, or charge decay, in conjunction with measurement of capacitance loading provides the appropriate way to assess the electrostatic suitability of materials . ‘Suitability’ being judged in terms of the avoidance of signiﬁcant surface voltage on a surface resulting from interaction with other surfaces or sources of charge. This method of assessment is more appropriate than traditional measurement of resistivity. Resistivity shows the fastest route by which charge can migrate over, or through, a material. Charge dissipation reveals the slowest route e and hence reveals the opportunity for charge to be retained and so maintain signiﬁcant surface voltages following tribocharging actions. A number of methods have been developed that aim to measure charge decay. Many of these are actually not suitable for assessing the suitability of materials and few either involve observation of the decay of tribocharge or have been shown to give results that match tribocharge decay [2,3]. The use of a high voltage corona discharge to deposit a localized patch of charge on the material to be tested and then a ﬁeldmeter to observe how quickly the surface voltage created decreases has been shown to be a versatile and practical way to assess materials . This method is described in Standards documentation .
E-mail address: [email protected]
URL: http://www.infostatic.co.uk http://dx.doi.org/10.1016/j.elstat.2014.06.001 0304-3886/© 2014 Elsevier B.V. All rights reserved.
While corona charge decay provides a method of measurement that can be easily be used on a wide variety of materials (including powders and liquids) the instrumentation involves appreciable mechanical complexity. To make measurements of decay times desirable for the effective limitation of static risks (well below 1 s) it is necessary to mount the corona discharge electrodes on a plate that shields the ﬁeldmeter from the corona voltages and yet can be moved away quickly so the ﬁeldmeter can observe the surface voltage created and its decay. Instrumentation that has been developed achieves removal of this shielding plate in about 20 ms and using a fast response ﬁeld mill ﬁeldmeter enables decay times to measured down to below 50 ms [4,6]. The present paper is concerned with an alternative method of measuring charge decay that does not involve the use of a high voltage corona and can be implemented within much simpler instrumentation. The method of measurement is described together with the results of preliminary studies on a number of materials. Comparative tests are also described based on corona charge decay and tribocharge decay measurements. 2. Induction charge decay measurement The basic arrangement for the new method for charge decay measurement is illustrated in Fig. 1. The ﬁeldmeter is positioned close to the surface to be assessed. The surface is supported with an open backing and is initially at earth potential. A step voltage is applied to the ﬁeldmeter. The localized electric ﬁeld created by the voltage difference between the ﬁeldmeter and the surface causes charge to migrate across, and perhaps through, the sample surface.
J. Chubb / Journal of Electrostatics 72 (2014) 396e401
Fig. 1. Arrangement for induction charge decay testing.
The basic form of the ﬁeldmeter response is illustrated in Fig. 2. There is an initial fast step in the ﬁeldmeter response followed by a slower rise towards the level that would apply if the sample surface were a fully conducting earthed surface. The size of the initial fast step in the ﬁeldmeter response is partly due to the ﬁeld created at the sensing aperture in relation to its structural earthed surroundings and partly to the dielectric constant and any very fast charge migration features in the sample surface e such as, for example, conductive threads in specialized fabrics. The form of the slower change of ﬁeldmeter output after the initial step reﬂects the rate and character of the charge migration across and through the sample surface. It is this feature that is relevant to assessment of the suitability of materials and is the feature to be examined. The main prospective advantages of this approach in comparison to corona charge decay measurement are:
a) the avoidance of the need for the mechanical arrangements for fast removal of the ﬁeldmeter shielding plate carrying the corona discharge points b) avoidance of the need for as high voltages as needed for creating suitable corona discharge charging c) opportunity, with a fast response ﬁeldmeter, of measuring much shorter charge decay times than is feasible in corona charge decay d) avoidance of any inﬂuence of residual air ionisation. The main prospective limitations are: - the need for the ﬁeldmeter signal processing circuits to be stepped in voltage with transfer of observations back to any ground level data analysis, storage and display facilities
Fig. 2. Response of ﬁeldmeter to step function application of voltage. (Picoscope record of 600 V induction charging test on taut surface of blues fabric 20140322-0001).
J. Chubb / Journal of Electrostatics 72 (2014) 396e401
- the lower electric ﬁelds likely to be available for measurement with certain materials requiring higher signal to noise performance from the ﬁeldmeter. In particular this will limit the opportunity to study charge decay on samples with an earthed backing and with close patterns of embedded conductive threads e which are desirable capabilities . The above approach may appear to have similarities to IEC11493  but is signiﬁcantly different. The most important differences are a) that the induction charge decay method induces charge and makes observations for the same side of the surface to be tested, and b) that the main function of IEC1149-3 is to assess the shielding capabilities of materials. (An alternative approach for assessing shielding performance has been developed and described ). An approach based on signal decay after exposure to a limited period of induction charging is not an appropriate as a general method for assessing the suitability of materials . The reason is, of course, because features where charge migration is very slow may not become fully charged, so they are not fairly assessed. 3. Experimental arrangements for testing 3.1. Arrangements for induction charge decay testing The performance of the induction charge decay approach described was examined using the set up illustrated in Fig. 1. A JCI 140 Static Monitor  was used as a ﬁeldmeter. The signal output on the sensitivity range used for induction charging studies was 1.0 V output for an electric ﬁeld of 23 kV m 1 at its sensing aperture. For the tribocharging a sensitivity a tenth of that was used. The ﬁeldmeter response time was 3 dB at 100 Hz. The ﬁeldmeter was mounted on insulation down from the top of an earthed shielding enclosure 200 mm diameter at its lower end. The base of this shielding enclosure rested on the surface of the sample to be tested. The gap between the sensing aperture of the ﬁeldmeter and the plane of the sample surface was 20 mm. Beneath the sample was 150 mm diameter open aperture earthed support surface for supporting and earthing the boundary of the sample. The ﬁeldmeter was linked to a Picoscope 3224 digital oscilloscope that was linked to an Apple MacBook laptop computer.
Observations were displayed and recorded using Picoscope 6 software running within a partitioned Windows XP operating system. The MacBook was run on its batteries (for electrical isolation) and the Picoscope was powered via its USB link to the MacBook. The Picoscope and computer were supported on a metal tray that was stood off from the bench surface to keep its capacitance to ground low. The ﬁeldmeter and the support tray for the Picoscope and computer could be quickly stepped up in voltage from earth by switching connection from earth to the output of a Monroe Model 214 high voltage supply unit that provided voltages of either polarity to be applied in steps of 1 V, 10 V, 100 V and/or 1000 V up to ±3 kV. For the induction charge decay studies a voltage of 600 V was used and with the particular ﬁeldmeter geometry used this gave an electric ﬁeld about 35 kV m 1 at the ﬁeldmeter sensing aperture with an earthed metal sample surface. No control was available for the temperature and humidity of the test environment. To minimise risk of change in material characteristics in comparative tests between induction, corona and tribocharge decay measurements these tests were made soon after each other with some interlacing to examine consistency in performance. Care was also taken to minimize handling of test areas and to avoid breathing on to sample surfaces. For each period of induction charge decay testing the step voltage applied was kept stable at a deﬁned value. Observations were recorded of the ﬁeldmeter response in the absence of any test sample and when a metal conducting surface was used. These observations provided the reference signal levels. With some samples it was practical to pursue testing of until they reached an asymptotic level, as illustrated in Fig. 2. Where this was not practical measurements with the fully conducting surface provided the end point reference for pursuing decay time calculations. 3.2. Arrangements for corona charge decay testing Corona charge decay measurements were made using a JCI 155v5 Charge Decay Test Unit [3,6]. Samples were supported in a JCI 176 Charge Measuring Sample Support. This provided the facility to measure the corona charge transferred to the test surface and from
Fig. 3. Analysis of decaying portion of induction charge decay with cling ﬁlm. Time to 1/e about 70 ms.
J. Chubb / Journal of Electrostatics 72 (2014) 396e401
this the capacitance loading could be calculated [3,11]. Observations were analysed and displayed using JCI-Graph software . 3.3. Arrangements for tribocharge decay testing Tribocharge decay tests were carried out with the same basic arrangement as used for the induction decay tests with one side of the shield lifted so the central region of the fabric could be touched or lightly impacted with a woolen sock tightly wrapped around the handle of a thin wooden spoon that was then quickly withdrawn. The arrangement was similar to that used in earlier studies . 3.4. Sample materials Three sample materials were tested: a cotton handkerchief, an area of cling ﬁlm and an area of blue artiﬁcial fabric. Each sample was tautly supported to minimize the risk of movement of the sample surface during a test due to electrostatic attraction to the ﬁeldmeter. The ambient humidity over the period of testing was quite high e 65e75% and not necessarily constant during any one day. This limited the range of testing opportunities and consistency of results with the materials readily available.
Attempts were made to test a sample of a cleanroom garment fabric with a 5 mm stripe pattern of included conducive threads. While corona charge decay tests indicated decay times that would have been useful, the high capacitance loading provided by the conductive threads meant that the voltage for the start of decay was too close to the maximum of that for a metal surface for sensible measurements. This illustrates one feature limiting application of induction charge decay measurements. 4. Test results Induction charge decay observations were analysed by transferring the Picoscope data, recorded as .csv ﬁles, into an Excel spreadsheet with observations displayed as a graph of ﬁeldmeter output voltage versus time. Examples of induction and corona charge decay graphs for cling ﬁlm are shown in Figs. 3 and 4. The voltage and the time for the start of the induction charge decay were taken as that at the beginning of the smooth part of the rising signal, after the initial fast rise e as indicated in Fig. 2. The end point voltage was taken as that provided by observations with a ﬂat metal sample surface. The 1/e and the 10% voltage decay levels were then calculated as fractions of this difference and these values and associated times found in the spreadsheet list of ﬁeldmeter
Fig. 4. Corona charge decay measurements with cling ﬁlm and analysis.
J. Chubb / Journal of Electrostatics 72 (2014) 396e401
voltages. The values obtained for the 3 samples tested are shown in Tables 1e3. Tribocharging observations were analysed in basically the same way as the induction charge decay observations. It was only practical to make tribocharging measurements with the blue fabric because decay times with the cling ﬁlm and cotton surfaces were too fast compared to the time for charging, removal of the charging surface and resetting the position of the shield mounting the ﬁeldmeter. Results for the blue fabric are shown in Table 1. Corona charge decay observations were analysed using the software JCI-Graph to obtain decay times to 1/e and to 10%. Examples of decay curves for cling ﬁlm are shown in Fig. 4. 5. Discussion on results The results for the three materials tested in Tables 1e3 show there are differences in charge decay times between the three methods of test. In particular: - Induction charge decay measurements with the blue fabric seem broadly comparable to tribocharge decay results but both are deﬁnitely longer than decay times measured by corona charge decay. - With cling ﬁlm induction charge decay times are deﬁnitely shorter than decay times measured by corona charge decay e particularly to the 10% end point level. - With the cotton fabric decay times seem more comparable between induction charge decay and corona charge decay. - Each set of measurements was fairly self-consistent. Variations between days may well have been due to charge of humidity and/or different areas of sample tested. Direct comparison between the three methods of charge decay testing is not simple. The delay between the end of charging and the time at which the voltage is taken for the start of the decay is a bit different between the three methods. This may affect calculation of decay times because the rate of decay usually slows up progressively during the progress of charge decay. With induction charging the decay starts within a ms or so of application of the charging voltage. With corona charge decay there is the delay of about 20 ms between the end of corona charging and the peak signal observed. (This is due to the time needed for the plate carrying the corona discharge points and shielding the ﬁeldmeter to move fully out of the ﬁeld of view). With tribocharge decay there was about a ½ s delay between the end of charging and observation
of the peak voltage, associated with the time needed to remove the charging surface and seat the ﬁeldmeter and shield back down on the surface. In the studies with the blue fabric an attempt was made to examine if this delay would signiﬁcantly affect results calculated for the corona charge decay tests. For the analysis in JCI-Graph a delay of 0.5 s was introduced between the end of charging and the selection of the decay timing start. The results are shown in the right hand pair of columns in Table 1. While these show a delay in the start of decay timing gives longer decay times it is clear that corona decay times remain deﬁnitely shorter than induction and tribocharge decay results for the blue fabric. Differences between the three methods of testing might arise if there is some difference in the species of charge migrating with the different methods of charging, if there is difference in the microscopic distributions of charge at the surface or if there is any inﬂuence from the area charged and the area of the sample. The response time of the ﬁeldmeter did not have any inﬂuence in the present studies because this time is short compared to all the other times involved e as shown by the fast initial rise of signal in the induction and corona charge decay tests. It would be useful to pursue comparison between charge decay performance from induction, tribo and corona charging with a wider variety of materials. This could be relevant to the development of Standards. The approaches of scuff and ball dropping charging may be useful for achieving quick response and good quality measurements in tribocharging studies [3,12]. 6. Comments on practical application The method of induction charge decay described provides a simpler way to assess the characteristics of materials than tribo or corona charge decay. It is however not as generally applicable as the corona charge decay method. One basic limitation is that the level of the ‘zero’ signal to be used in assessing decay curves is not as simply deﬁned. For a plane sample surface (for example a stretched area of fabric) the ‘zero’ can be well deﬁned by measurements using a plane conducting sample surface. This deﬁnes the level to which the ﬁeldmeter readings will eventually rise during ‘decay’. With non-plane surfaces it is not as easy to establish this end point ‘zero’ unless one can feel sure that the decay has reached an asymptotic top level. With corona and tribocharge decay the zero is deﬁned by the zero of the ﬁeldmeter, which can be determined just before each test and checked independently. When studying light ﬂexible materials it is necessary to ensure these are held taut to reduce the inﬂuence of movement of the
Table 1 Artiﬁcial ﬁbre blue fabric. Test reference
Induction charge decay
Corona charge decay From peak
40346 (22/03/14) 20140322-001 20140322-004 20140322-005 20140322-006 40347 (22/03/14) 40348 (22/03/14) 20140322-0007 40361 (28/03/14) 40362 (28/03/14) 20140328-0001 20140328-0002 20140328-0003 20140328-0004 40363 (28/03/14)
34 36.5 40.5
With 0.5 s delay
165 152 150
71 74 96 94
J. Chubb / Journal of Electrostatics 72 (2014) 396e401 Table 2 Cling ﬁlm. Test reference
40339 (17/03/14) 40340 (17/03/14) 40349 (22/03/14) 40350 (22/03/14) 40351 (22/03/14) 40354 (25/03/14) 20140325-0002 40356 (25/03/14) 20140325-0003
Induction charge decay
Corona charge decay
0.062 0.061 0.085 0.056 0.051 0.054
Table 3 Cotton handkerchief. Test reference
Induction charge decay (s)
Tribocharge decay (s)
Corona charge decay (s)
20140326-0001 20140326-0002 20140326-0003 40359 (26/03/14) 40360 (26/03/14) 20140326-0004 20140326-0005
0.022 0.021 0.020
0.055 0.053 0.052 0.014 0.014
B Induction charge decay results with a blue fabric artiﬁcial ﬁbre fabric are comparable to tribocharge decay results, but are longer than measurement from corona charge decay. B Induction charge decay times with cling ﬁlm are deﬁnitely shorter than decay times from corona charge decay. B Results with the cotton fabric show similar decay times between induction charge decay and corona charge decay. Induction charge decay is not proposed as a replacement for corona or tribocharge decay testing. The deﬁnitive test remains tribocharge decay measurement, but this is often not practical or convenient and involves more difﬁcult experimental test arrangements. Induction charge decay measurement does offer the opportunity for simpler instrumentation, opportunity to measure faster charge decay times and avoids any inﬂuence of air ionization. It is concluded that the induction charge decay method of testing materials described warrants fuller investigation e in particular regarding apparent differences in charge decay behaviour between induction, tribo and corona charge decay measurements. If conﬁrmed, these differences are relevant to the deﬁnition of Standard methods of test for assessing the suitability of materials. References
sample surface under electrostatic attraction. Any movement of the sample surface as the electric ﬁeld between the sample and the ﬁeldmeter decreases could affect the effective ‘zero’ level. Such problems do not arise in tribo or corona charge decay measurements where there is a larger separation distance between the sample surface and the ﬁeldmeter e so electrostatic forces are much smaller and the ‘zero’ is well deﬁned by a zero initial charge condition. As much lower voltages are used in induction charge decay measurements than in corona charge decay the ﬁeldmeter signals will be much smaller. This means that decay time measurements to a 10% end point level require a ﬁeldmeter with particularly good signal to noise ratio and the use of an appropriate technique for accurate time measurement in the presence of signal noise (for instance stutter timing ). 7. Conclusions The method of induction charge decay testing described has been shown to produce fairly consistent results in repeat tests with each of the three materials tested. Comparison of results with the limited range of materials tested with induction, corona and tribocharge decay measurements indicate:
 J.N. Chubb, I. Pavey, Assessing the Electrostatic Suitability of Materials, J. Electrostatics Society of America Meeting Cambridge, Ontario, Canada, June 12e14 2012.  J.N. Chubb, Measurement of tribo and corona charging features of materials for assessment of risks from static electricity, IEEE Trans. Ind. Appl. 36 (6) (Nov/Dec 2000) 1515e1522.  J.N. Chubb, Experimental Comparison of the Electrostatic Performance of Materials with Tribocharging and with Corona Charging. http://www. infostatic.co.uk/cache/Tribo-corona-comparison.pdf.  J.N. Chubb, Instrumentation and standards for testing static control materials, IEEE Trans. Ind. Appl. 26 (6) (Nov/Dec 1990) 1182.  IEC 61340-2-1, Electrostatics e Part 2-1: Measurement Methods e Ability of Materials and Products to Dissipate Static Electric Charge, 2002 (update due end 2014).  http://www.infostatic.co.uk/Leaﬂets/JCI155v5.pdf.  IEC/TS 61340-4-2, Electrostatics Standard Test Methods for Speciﬁc Applications. Electrostatic Properties of Garments, 2013.  J.N. Chubb, Non-contact measurement of the electric ﬁeld shielding performance and the resistivity of layer materials, J. Electrost. 64 (2006) p685e689.  J.N. Chubb, Comments on methods for charge decay measurement, J. Electrost. 62 (2004) p73e80.  http://www.infostatic.co.uk/UM/UM140.pdf.  J.N. Chubb, An Introduction to Electrostatic Measurements, Nova Publishers, 2010, ISBN 978-1-61668-251-4.  J.N. Chubb, Tribocharging studies on inhabited cleanroom garments, J. Electrost. 66 (2008) p531e537.  J.N. Chubb, J. Harbour, I. Pavey, Stutter Timing for Charge Decay Measurement, ‘Electrostatics 2011’ IoP Conference, Bangor, April 2011. IoP Conference Series 301, 2011.